Characterization of lithium fluoride windows at 450 K for shock
wave experiments: Hugoniot curves and refractive index
at 532 nm
E. Fraiziera, P. Antoine, J.-L. Godefroit, G. Lanier, G. Roy, and C. Voltz
CEA Valduc, 21120 Is sur Tille, France
Abstract. Lithium fluoride (LiF) windows are extensively used in traditional shock wave experiments because of their transparency beyond 100 GPa along  axis. A cor-rect knowledge of the optical and mechanical properties of these windows is essential in order to analyze the experimental data and to determine the equation of state on a large variety of metals. This in mind, the windows supply is systematically characterized in order to determine the density, the thermal expansion and the crystalline orientation. Fur-thermore, an experimental campaign is conducted in order to characterize the windows properties under shock loading at 300 K and preheated conditions (450 K). This article describes the experiments, details the analysis and presents the results. Particle velocity measurements are carried out at the interface of a multiple windows stack using inter-ferometer diagnostic (VISAR and IDL) at 532 nm wavelength. Shock velocity is calcu-lated as a function of the time of flight through each window. The optical correction is calculated as the ratio of the apparent velocity gap and the particle velocity at the free surface. To go further, the Rankine-Hugoniot relations are applied to calculate the pres-sure and the density. Then, the results and uncertainties are presented and compared with literature data.
1 Challenges for the LiF characterization
Traditional shock wave experiments need windows to characterize a variety of materials. Lithium flu-oride (LiF) is extensively used for that purpose because it remains optically transparent until more than 100 GPa. In order to analyse and simulate the experiments it is necessary to have a good knowl-edge of the optical and mechanical properties of these LiF windows. This in mind it is necessary to characterize our windows supply: density, crystalline orientation, acoustic velocity and dimensional measurements. Furthermore, a campaign is conducted in order to characterize the behaviour under dy-namic loading in particular at 450 K which is the selected temperature level for some of our preheated experiments .
2 Experiments principle and campaign
Under classical impact configuration the optical diagnostics measure the velocities at the interfaces (Fig. 1).
First of all, the shock wave time of flight ΔtLiF is measured at the interface and at the free sur-face with the VISAR. Knowing the thickness eLiF of the LiF window, the shock wave velocity US is
FS u LiF
FS u LiF
Fig. 1. Principle of the experiments and velocities diagnostics.
Fig. 2. Experimental assembly scheme and quarter coated windows.
Secondly, relations from literature [2–7] allow to determine the optical corrective index n0−λfrom the ratio of the apparent velocity gapΔua(when the shock emerges at the free surface) and the velocity
at the free surface uFS.
The actual particle velocity upat the interface is consequently determined (3).
To go further, the Rankine-Hugoniot relations are applied. The pressure is then calculated (4) and the shock density is expressed as a function of the initial densityρ0, the shock velocity US and the particle
Finally, the refractive index n is determined as a function of density (6).
0 500 1000 1500 2000
2200 2400 2600 2800 3000 3200 3400
Vi te ss e ( m . s -1 ) V1 V2 V3 Ta/LiF impact a
ΔLiF/LiF gap Velo cit y (m/s) Time (ns) 0 500 1000 1500 2000 Vi te ss e ( m . s -1 ) V1 V2 V3 Ta/LiF impact a
ΔLiF/LiF gap Velo cit y (m/s)
Fig. 3. VISAR diagnostic of the interfaces velocities.
at the diﬀerent interfaces. The pressure ranges from 7 to 21 GPa using tantalum flyer and buﬀer. A computer simulation enables to predict the pressure and the velocity diagrams in order to adjust the optical diagnostics.
The LiF supplies (from BFI OPTILAS) are characterized to determine the following values:
•  for the crystalline orientation,
• 2.630 for the density at 300 K,
• α = 3.990×10−11 ×T2+5.125×10−8×T +3.225×10−5μm.m−1.◦C−1for the linear thermal expansion along the  axis .
• 6396 m.s−1for the longitudinal acoustic velocity along the  axis.
The preheated system is calibrated on LiF apparatus with 6 temperature measurements. The homo-geneity is less than 10 K on a window. Furthermore a computer thermal simulation (Fluent code) confirms these results.
3 Experiment analysis at 450 K and 20.4 GPa
This part presents the analysis of the VISAR results (Fig. 3) at the interfaces for the experiment con-ducted at 450 K and 20.4 GPa. The DLI measurements enable to check the apparent velocity using a second diagnostic.
Gaps in the assembly produce visible eﬀects on velocity profiles. The velocity measured (without optical correction) on the tantalum buﬀer shows its free flight (46 ns) before the impact on the first LiF window. Furthermore, a local decrease of velocity corresponds to the gap between the two windows.
When the shock emerges at the free surface the classical velocity gapΔuais observed.
The first exploitation consists in the measurement of the shock time of flightΔtLiFin the two
win-dows. The shock velocity is calculated, knowing the thickness of both LiF winwin-dows. Then, the velocity plateau and the velocity gap when the shock emerged at the free surface are measured. Furthermore, the free surface velocity is also measured and the relation (2) is applied in order to determine the cor-rective index. At least, the Rankine-Hugoniot relations enable to calculate the shock pressure, density and refractive index (4–6).
5000 5500 6000 6500 7000 7500 8000
0 200 400 600 800 1000 1200 1400 1600 1800
up (m.s -1
LaLone08 Jensen07 Lalle87
This study acoustic VL SESAME 300K SESAME 450K This study 300K This study 450K
Fig. 4. Shock velocity as a function of the particle velocity.
the uncertainties calculation (and unfortunately their propagation). So, with experimental uncertainties of roughly 2% the calculated values reach more than 4–6% of uncertainties.
Δ(a×b) a×b =
Δ(a/b) a/b =
Δa a +
Δ(a+b)= Δ(a−b)= Δa+ Δb (8)
4 Experimental results
The Fig. 4 represents the shock velocity (1) as a function of the particle velocity (2–3). Our results are compared to the literature data at ambient temperature. They are in good agreement with the results from Lalone  and Lalle [6, 7] but show strong deviation from Jensen data . Furthermore, the SESAME data (dashed lines) are consistent with our uncertainty level at ambient temperature and at 450 K. The initial temperature dependence is evident and a decrease of the shock velocity is observed for the preheated experiments.
To go further, the pressure and density are calculated. The refractive index is then calculated from the relations (2) and (6). Furthermore, the density is normalised with the initial densityρ0(T ) corre-sponding to the initial temperature of the experiment. Applying the measured linear expansion (along  axis), with the first approximation of an isotropic material, the calculated density at 450 K is 2.582. Once again our results are in better agreement with data from Lalone  than from Jensen . As for them, a linear fit taking our uncertainties into account is achieved (9).
1,39 1,40 1,41 1,42 1,43 1,44
1 1,05 1,1 1,15 1,2 1,25 1,3 1,35 1,4
Lalone08 Jensen07 Lalle87 (@514nm) This study 300K This study 450K
Fig. 5. Refractive index as a function of the normalized density.
Nevertheless, diﬀerences with the study of Lalle [6, 7] realized at 514 nm are also explained be-cause the refractive index is a function of wavelength.
Finally, a further study is necessary to measure directly the density as a function of temperature. Indeed, the LiF has a crystalline orientation and the application of the linear expansion (isotropic approximation) could be discussed and improved in future works.
5 Conclusions and future works
The present work is in good agreement with literature data at ambient temperature. Few diﬀerences could be explained by diﬀerent supplies and initial density used. Furthermore, the optical and mechan-ical characterization conducted under shock at 450 K enables a better interpretation of our preheated experiments on a variety of materials.
Taking into account the initial temperature through the initial density, our results confirm the theory that the refractive index is a linear function of the normalized densityρ/ρ0 and a 1.2926±0.1263 corrective index is obtained. The preliminary characterization of the LiF windows is a key point and the initial density merits a particular attention.
So, a future work is planned to measure the windows density at the initial temperature of our experiments. Furthermore, the uncertainties need to be improved for a better interpretation of the ex-periments involving window. For that purpose, simplified target configurations seem to be a promising way. A new campaign should also be conducted for the shock and optical characterization of sapphire windows.
1. G. Roy and al, BAGHEERA: A new experimental facility at CEA/Valduc for actinides studies under high dynamic loading, J. Phys. IV France 134, pp. 731-737, (2006).
4. D.R. Goosman, J. Appl. Phys. 65, (1989).
5. J. Wackerle, H.C. Stacy and J.C. Dallman, Pro. Inst. Soc. Opt. Eng (SPIE) 832, 72 (1987). 6. P. Lalle, Internal report CEA, (1987).
7. P. Lalle, Internal report CEA, (1997). 8. O. Duret, Internal report CEA, (2009).
9. B.M. Lalone, O.V. Fat’yanov, J.R. Asay and Y.M. Gupta, Velocity correction and refractive index
changes for  lithium fluoride optical windows under shock compression, recompression, and unloading, Journal of applied physics 103, (2008).
10. B.J. Jensen, D.B. Holtkamp, P.A. Rigg, D.H. Dolan, Accuracy limits and window corrections for